Observation of structural, optical, electrical and magnetic properties of ternary copper-doped CeO2/GO/SrTiO3 nanocomposites

A ternary system involving copper-substituted ceria (Cu:CeO2)0.95−y(GO)y(SrTiO3)0.05 nanocomposite where the GO concentration (y) is varied between 0.15 and 0.30. The innovation of this work lies in the purposeful assembly of the nanocomposite using a grinding method, which was optimized through the individual fabrication of Cu-doped CeO2 with different CuO concentrations. In the first, Cu-doped CeO2 with various CuO concentrations (x = 0.0, 0.05, 0.1, 0.2, and 0.3) was first individually fabricated based on a sol–gel auto-combustion strategy to optimize the best ratio. The XRD profiles confirm the successful fabrication of cubic cerium (IV) oxide CeO2 using glycine as a fuel at an annealing temperature of 400 °C for 2 h. AC conductivity was investigated for both Cu-doped CeO2 and the ternary nanocomposite over a wide frequency range (10–1 to 107 Hz) at room temperature. The conductivity showed lower values for CeO2 doped with 0.05, 0.2, and 0.3 wt% CuO, whereas it showed its maximum values upon doping with 0.1 wt% CuO. Interestingly, the conductivity of graphene oxide–doped CeO2 was 103 times higher than that of pure CeO2, i.e., it increased from 1.7 × 10–6 to 2 × 10–3 S/cm. The magnetic-field dependence of MS of the ternary Cu-doped CeO2/GO/SrTiO3 nanocomposites showed a systematic increase in MS as the Cu2+ ion content increased. This strengthens the ferromagnetism in our samples as Cu2+ ion content increases.


Introduction
Solid oxide fuel cells (SOFC) are promising power generators that directly convert chemical energy to electricity with low emission and high efficiency, making them a major clean energy conversion technology in the future [1][2][3]. Typically, the cell consists from three main parts: anode, cathode, and electrolyte, but the anode has the most vital role in controlling the overall performance [4,5]. The anode enriches the oxidation process of the fuel, electrical transport of electrons, and transport of by-products of the electrochemical reaction. Therefore it should have great catalytic activity, moderate electrical conductivity, chemical compatibility, and matching with other SOFC components [6][7][8]. However, there are limitations to be overcome in the commercialization of SOFC, primarily due to the lack of optimal anode materials for high temperature operation (600-900°C), the region where efficiency is maximized [2,9]. For instance, the Ni-based cermet anode has high catalytic activity and electrical conductivity at high temperatures. However, the Ni-based electronic conducting network in these anodes can be disrupted by repeated cycling of redox reactions and easy oxidation associated with the coarsening and aggregation of Ni particles. Since that, searching for new functional anode material has been indispensable [10].
To minimize the oxidation and overcome the stability limitations, Ni alloyed with transition metal elements as Co rather than using pure Ni has been introduced. Although alloying has improved durability, cobalt is classified as a critical raw material, i.e., an element of high economic importance but limited supply [11]. Also, oxide anode has drawn much attention for years. Perovskite materials such as doped LaCrO 3 , doped SrTiO 3 [12][13][14], and the double perovskite materials Sr 2 Mg 1-x Mo x O 6-d [15] have been developed as SOFC anodes. However, the electronic conductivity of these doped oxides is only on the orders of 1 S/cm under SOFC anode conditions, and the double perovskites are reported as unstable in reducing atmosphere above 900°C [16,17]. However, due to the dual magnetic and electrical natures of some of these compounds as SrTiO 3 , the alignments of magnetic dipole moments helps to increase effective ionic conductivities and diffusivity.
Recently, Cu-doped CeO 2 has been reported as a stable ceria-based anode material with higher catalytic activity for carbon gasification and electrical conductivity than pure CeO 2 . However, this latter needs to be at least one order of magnitude larger for SOFC applications [18]. Improved performances have been obtained by developing composite electrodes of transition metal oxides and graphene. Graphene has almost no bandgap and exhibits remarkable electrical and optical characteristics such as high carrier mobility (2 Â 10 5 cm 2 /V s), high conductivity, unique structure, high mechanical strength, thermochemical stability, and high transparency (* 97.7%) [16,17,19,20].
The key idea of the present study is to develop a new functional anode based on the combination of materials with optimized properties to maximize electrical conductivity and enhance durability as well. For that, we have developed, for the first time, a series of (Cu:CeO 2 ) 0.95-y (GO) y (SrTiO 3 ) 0.05 nanocomposite where (y = 0.15, 0.25 and 0.30) by sol-gel combustion and ball-milling method. To enhance ionic polarizability, SrTiO 3 was selected in this study due to its high redox stability and improved performance for fuel oxidation. At the same time, graphene is chemically compatible with SrTiO 3 -based electrodes and exhibits high ionic conductivity. Moreover, the perovskite is A-site-deficient and alkalineearth-free to prevent possible superficial phase segregation. The nanocomposite electrodes were studied by various structural, microstructural, magnetic, and electrical techniques to evaluate their potential use as fuel electrodes in solid oxide cells.

Preparation of SrTiO 3 nanopowder
Anhydrous strontium nitrate was treated with titanium oxide powders in an aqueous solution. Glycine was incorporated into the solution. After that, hydrogen peroxide (10%) was added to the solution to enhance the reactivity of the starting materials. The produced suspension was heated on the hot plate magnetic stirrer until dry. Afterward, the formed powders were dried entirely at 100°C overnight in an oven. Finally, the formed precursor sample was thermally annealed at 1000°C for 2 h at the temperature control of 10°C/min in a static air atmosphere muffle furnace.

Preparation of Cu:CeO 2 /GO/SrTiO 3 ternary composite
To produce ball-milled ternary nanocomposite, different materials with various ratios given in Table 2 were placed in 130 cm 3 agate jars using four 1.5 cm zirconium spheres in a ball mill weighing 25 g. The ball mill equipment was then run for 2 h at 450 rpm [21]. The resultant ball-milled samples were labeled with Composite 1, 2, and 3.

Physical characterization
X-ray diffraction profiles differentiated the formed products' phase formation based on a Brucker D8advance using Cu K radiation (k = 1.5406) with a typical scan range of 2°from 20°to 80°and a scan rate of 2h/min. The crystallite size of copper-doped CeO 2 nanoparticles was obtained utilizing the Debye-Scherrer formula to determine the X-ray diffraction data [22,23]: where D is the crystal size, K = 0.9 is a correction factor used to account for particle morphologies, FWHM (full width corrected at half maximum) is the peak's measurement, the wavelength is the measurement, and Bragg angle is the measurement. Transmission electron microscope (JEOL, JEM-1230) operating at 80 kV. A transmission electron microscope (JEOL, JEM-1230) operating at 80 kV was established to assay the synthesized samples' microstructures. The Fourier transform infrared spectroscope (FTIR) was realized using Japan's Jasco JASCO 3600 spectrophotometer. Raman spectra were collected using a confocal Raman microscopy system (LabRAM HR evolution, Horiba Scientific) under excitation with a 532 nm laser. For AC conductivity (rac) measurements, the disc-shaped sample was placed between the two electrodes of the measuring cell connected to the broadband dielectric spectroscopy (BDS), Novo control, Germany. The r ac was carried out over a wide frequency range (10 -1 to 10 7 Hz) at room temperature (RT). The r ac was carried out over a wide frequency range (10 -1 to 10 7 Hz) at RT and given as a function of the frequency of the applied electric field (f) and the dielectric loss (e''): where e o = 8.85 9 10 -12 F/m is the permittivity of the vacuum. The error in e'' amounts to ± 1%. The reproducibility of the measurement was tested by remeasuring r ac and e'' after experimenting once again. The vibrational sample magnetometer (VSM) model, Lake Shore model, 7400 VSM, US, Lake Shore Co., Ltd. Ltd., USA, was employed to measure the magnetic characteristics of the produced samples in an applied magnetic field 20 KOe at RT.

Cu-doped CeO 2
In this study, the sol-gel technique made numerous CeO 2 samples based on Cu doping. To optimize the best ratio, these samples' structural characteristics were described using a different molar ratio of (x = 0.0, 0.05, 0.1, 0.2, and 0.3). Figure 1a manifests the XRD forms of Ce 1-x Cu x O 2 (x = 0, 0.05, 0.1, 0.2, and 0.3) tailored based on an auto-combustion method using sol-gel using glycine as a fuel annealed at 400°C for 2 h. Plainly, All the composed peaks referred to CeO 2 as cubic phase according to (JCPDS no. 81-0792) [24]. The diffraction lines related to the lattice planes (111), (200), (220), and (311) facets at 28.5°, 37.3°, 47.5°, and 56.6°are assigned. However, Cu 2? substitution indicates a noticeable decrease in CeO 2 crystallinity [25]. The crystallite size of the synthesized powders was evaluated from the highest using (Debye-Scherrer's equation), the craziest peak (111) of the cerium oxide phase. It was found to be 13 nm for pure CeO 2 . However, the crystallite size was decreased by the addition of Cu 2? ions. Meanwhile, the crystallite size was increased by further incrementing the Cu 2? ion content. The results imputed that the ionic radius of the Cu 2? ion (0.73 Å ) was lower than the ionic radius of the Ce 4? ion (1.01 Å ) [26]. The unit cell volume and the lattice constant of Cu subrogated CeO 2 were decreased as a Cu 2? ion with a smaller radius was inserted into CeO 2 as the result of a contraction of the lattice happened to cause a decrease in the lattice constant. The change in structural parameters is recorded in Table 3. The Williamson-Hall equation can estimate the crystallite size as predicted in the previous references [27,28]. Accordingly, the estimated values of D using the Williamson-Hall equation are presented in Table 3. The D value calculated using the Williamson-Hall method is higher than that obtained using the Scherrer equation, where the Williamson-Hall equation considers all diffraction peaks and assumes the brooding of it. That is related to the crystalline size and the lattice strain, which is not considered in the Scherrer equation. The considerable value of D from Williamson-Hall for the 0.30 ratio of Cu-doped CeO 2 may be attributed to the large lattice strain due to adding a high percent of Cu.
The microstructure Cu-doped CeO 2 nanoparticles are considered by the TEM technique, as given in Fig. 2. The sample of pure CeO 2 demonstrates aggregated, nearly well-dispersed spherical NPs with narrow diameters from 4 to 11 nm. The SEAD rings showed the diffraction patterns related to a polycrystalline characteristic of cubic CeO 2 was indexed.
With an increment of Cu substitution content to 10%, the particle size with the narrow diameters decreased from 2 to 6 nm with a quasi-spherical-like structure. Further, an increase in Cu content to 30%, more agglomeration of the spherical particles, augmenting the particle size to 3-10 nm. However, SEAD patterns  Figure 3a shows diffuse reflectance (DRS) spectra in the wavelength range of 220-2000 nm for pure and Ce 1-x Cu x O 2 (x = 0, 0.05, 0.1, 0.2, and 0.3) samples. As a direct charge transfer, the CeO 2 spectrum exhibits the absorption peak at 340 nm at the transition between the O-2p and Ce-4f bands. The reflectance spectrum was changed as the absorption edge shifted to the higher wave number, red-shift, after adding Cu 2? ion. An interfacial polaron effect may cause the red-shift by electron-phonon interaction [29].
where light reflectance is denoted by R, the absorptions (a), and scattering coefficients (S). Another factor, like constant (A), relies on the possibility of the transition. P is a direct or indirect band gap (2 or 1/2), respectively. The E g values of Cu-substituted CeO 2 nanoparticles have been assessed using the Kubelka-Munk absorption function for direct gap semiconductors [21,[32][33][34], evidenced in Fig. 3b and c. A linear correlation between (aht) 2 and ht reveals the direct transition nature of Cu-substituted CeO 2 . The band gap energy was discovered to diminish from 2.99 eV for pure CeO 2 to 1.00 eV for Ce 0.9 Cu 0.1 O 2 with a 10% Cu ratio substituted CeO 2 . The results can be discussed based on Cu 2? ions with lower ionic radius replaced e Ce 4? ions with bigger ionic radius and the modulation of the required energy for absorption. Subsequently, the Cu 2? ion with 10% content decreased in the band gap energy due to the red-shift for the synthesized as seen by (i.e., increased wavelength). The conductivity measured at RT for the Ce 1-x-Cu x O 2 (x = 0.0, 0.05, 0.1, 0.2, and 0.3) has been investigated first as a function of frequency and then as a function of the composition at a constant frequency value, i.e., 10 3 Hz. AC conductivity (r ac ) is a crucial electrical characteristic that controls how well a material conducts electricity when exposed to an electrical field [35,36]. Furthermore, an increase in the concentration and mobility of ions leads to a conductivity increase [37]. The AC's frequency dependency conductivity (r ac ) is most often represented by the Jonscher relation [38].
where A and s are constants, [r(x)] is the frequencydependent conductivity recorded with the AC field, and dc is the DC conductivity (r dc ). The lines of the conductivity vs. temperature plot are used to estimate the frequency exponent (0 \ s B 1), which uses for determining the conduction mechanism [39] as well as the modification of the glass network structure [40]. Generally, Several low-mobility amorphous and crystalline materials are covered by relation (3) [41]. Figure 4a and  showed the lowest value of E g and correspondingly the highest value of r ac, . Therefore, this composition Ce 0.9 Cu 0.1 O 2 will be chosen, and then we study the effect of introducing GO and/or SrTiO 3 and produce a ternary composite.

Cu:CeO 2 /GO/SrTiO 3 ternary composite
The composite here is fabricated from Ce 0.9 Cu 0.1 O 2 , GO, and SrTiO 3 . Figure 5a represents the XRD picture of graphene oxide synthesized based on the modified Hammer method [42]. The typical diffraction peaks appeared at 2h at approximately 12.08°w ith d-spacing = d = 7.31966 nm, indicating the typical GO peak. Meanwhile, the peak at 2h of 23.27°w ith d-spacing 3.81934 nm depicted that the graphite is totally oxidized. Figure 5a indicates the formed crystal structure of strontium titanate SrTiO 3 analyzed using XRD patterns synthesized using sol-gel auto-combustion pathway at 1000 C for 2 h. Obviously, peak intensities associated with cubic The results demonstrated the peaks corresponding to cerium oxide, graphene oxide, and strontium titanate. Figure 5c depicts the FT-IR spectrum of Cu-substituted CeO 2 nanoparticles from 500 to 4000 cm -1 . It is clear that the absorption peaks below 700 cm -1 in Each example demonstrate the Ce-O stretching mode, emphasizing the CeO 2 phase being present in all samples [43]. Meanwhile, the peak of absorption occurring at about 1400 cm -1 is related to the atmospheric CO 2 non-asymmetric stretching vibration. Meanwhile, the bands centered in all samples at 3000-3500 cm -1 are linked to the O-H vibration of moisture absorption. Meanwhile, the additional 1100 to 1700 cm -1 peaks are associated with Ce-O stretching [44]. Furthermore, Cu doping observed a slight shift in the absorption bands centers of CeO 2 . Figure 5c evinces FT-IR spectroscopy of ternary Cudoped CeO 2 /GO/SrTiO 3 nanocomposites at different stoichiometry ratios. The peak bands at 1000-1300 cm -1 and 1500-1630 cm -1 manifest the entity of C=O and C=C stretching GO vibrational bands, mainly in Composite 1. The prominent peaks correspond to the O-H vibration of water adsorption at 3000 to 3600 cm -1 . The band at 1400 cm -1 is assigned to the O-H vibration of graphene oxide. The stretching vibration C-O-C peak occurring at 1210 cm -1 of GO has been indexed [45,46]. Furthermore, the located peak positions at 2850-2915 cm -1 may be related to CH 2 and C-stretching vibration bands related to unburned glycine residue. Meanwhile, the observed central peak is located at 643 cm -1 , belonging to the Ti-O stretching vibrations of the SrTiO 3 phase in the composite [47]. The distinctive peak at * 540 cm -1 is that tall peak of SrTiO 3 connected to Sr-Ti-O stretching vibration. Furthermore, the absorption peaks at around 850 cm -1 are due to the existence of Ti-O 6 octahedron stretching of SrTiO 3 material in the composite. Finally, similar absorption peaks of Cu-substituted CeO 2 are also observed [48]. Figure 6a offers the RT Raman spectra of CeO 2 and Ce 0.9 Cu 0.1 O 2 measured within a 0-1000 cm-1 range. A first-order Raman peak (F 2g ) at 460 cm -1 was observed for each CeO 2 and Ce 0.9 Cu 0.1 O 2, which agrees with the previous reports [49]. It can be noticed that the intensity of F 2g peak for Ce 0.9 Cu 0.1 O 2 is lower than CeO 2, indicating the doping by Cu. On the other hand, Fig. 6b displays the Raman spectra of graphene and Composite 2. Apparently, two bands corresponding to the disorder-induced (D-band) and in-phase vibration of graphene (G-bands) were assigned at * 1350 and 1585 cm -1 for the GO [50]. At the same time, the main F 2g mode band was observed at 455 cm -1 , characteristic F 2g vibration of CeO 2 [51]. Meanwhile, Figure S1 shows the RT Raman spectra of SrTiO 3 with weak bands for cubic SrTiO 3 at 272, 541, and 794 cm -1 noticed, which the TO 3 , TO 4 , and LO 4 phonon modes can assign [52]. Raman spectra were used and presented in Figure S2 to identify the electronic interaction. The sharper peak represented the vibration mode of Ce-O at 460 cm -1 (F 2g ). The band was red-shifted from 460 to 454 cm -1 due to oxygen vacancies, which are linked to constitutional flaws brought on by the absorption of Cu inside the CeO 2 lattice, which is present and growing. Plainly, two bands concerning the disorderinduced (D-band) and in-phase vibration of graphene (G-bands) were assigned at * 1350 and 1585 cm -1 . The stretching vibration of sp 2 carbon atoms gives rise to the G band, which correlates with the firstdegree scattering of the E 2g mode, whereas the stretching vibration of sp 3 carbon atoms gives rise to the D band, which results in flaws and disorders. Raman characteristic peaks based on first order, which correspond to the phonon modes of TO 3 , TO 4 , and LO 4 (271, 543, and 795 cm -1 , respectively). At 271 cm -1 , the bending vibration of O-Sr-O has been detected. At 543 cm -1 , the Ti-O-Ti was noticed for bending vibration mode. At 795 cm -1 , the Ti-O stretching type vibration was noticed. Figure S2 displays TEM micrographs of SrTiO 3 and GO samples. It is clear that the microstructure of SrTiO 3 nanoparticles exhibited a cubic-like structure, as presented in Figure S2(a). The average grain size was in the range of 7-12 nm. The selected-area electron diffraction (SAED) pattern is described in Figure S2(b). The SAED rings ascribed the cubic SrTiO 3 phase was indexed. Figure S2(c) presents the microstructure of GO as a sheet-like structure with a large thickness, a delicate surface, and a rugged edge. SAED pattern in Figure S2(d) displays the diffraction ring related to (002) of the graphitic carbon. Figure 7 represents the morphology Cu-doped CeO 2 /GO/ SrTiO 3 nanocomposites at different materials content. The results manifest that the spherical-like nanoparticles of Cu-doped CeO 2 and cubic SrTiO 3 are well distributed on the graphene nanosheets' surface, as seen in Fig. 7a, d, and g. Figure 7c, f, and i describes the nanoparticle's size and distribution measurements. In this context, the average size was decreased with decreasing the graphene oxide content. The mean grain size was 21.4 nm for composite 1, whereas the primary grain size was 11.38 nm for composite 2, and finally, the grain size of composite 3 was found to be 8.76 nm. SAED patterns showed a clear ring without any distortion in the lattice planes. The SAED rings demonstrate the presence of cubic ceria structure and a more heterogeneous structure in which Cu-doped CeO 2 NPs and SrTiO 3 were dispersed, evidencing the interaction between ceria and SrTiO 3 with GO. Based on the SAED pattern given in Fig. 7b, e, and h, the crystallinity of the composite was changed relating to the insertion of GO material. Figure S3(e) displays the DRS of ternary Cu-doped CeO 2 /GO/SrTiO 3 nanocomposites in the 200-2000 nm wavelength range. Meanwhile, Cu-doped CeO 2 was shifted towards a high wavelength; as a result, the defects in the shape of vacancies in the oxygen were induced by the higher amount of graphene oxide around the Cu-doped CeO 2 particles. The absorption peak at 390 nm might be connected to the electrical charge from Ti's 3d orbital to its 2p orbital of O of SrTiO 3 in the composite. Owing to Cu-doped CeO 2 semiconductor was coupled with narrow bandgap SrTiO 3 and graphene oxide semiconductor in composite, which enhanced ability to absorb visible light. The GO exhibits a maximum absorption at 225 nm and a hump at 313 nm, which denote the n-p* transition of the C-O functional groups and the p-p* transition of the C-C bond. The band gap energy E g value of the composite at different concentrations is demonstrated in Figure S

The frequency dependence
To understand the response of graphene oxide (GO), SrTiO 3 , and CeO 2 compositions, their electrical conductivities profoundly are suggested to be represented at constant frequency value (10 3 Hz) in one graph as illustrated in Fig. 8a and listed in Table 5. Compared to CeO 2 compositions, GO exhibited the highest conductivity value (r ac = 10 -2 S/cm), whereas SrTiO 3 showed the lowest value (r ac-= 7.5 9 10 -9 S/cm). Since adding SrTiO 3 to the composite is planned to enhance the chemical stability, we must keep a minimum content of SrTiO 3 as low as 0.05 wt% into the composite to eliminate the possible increase in conductivity. Also, GO-doped CeO 2 showed much higher conductivity values than those doped with CuO; the duel composite of CeO 2 Fig. 7 TEM image, SEAD, and particle size distribution of a, b, and c for Composite 1. d, e, and f for Composite 2. g, h and i for Composite 3, respectively and 0.25 wt% GO showed a much higher conductivity than all Cu-doped CeO 2 composite samples. Figure 8b manifests the frequency-dependent conductivity of the pure CeO 2 in comparison with that recorded for the graphene oxide (GO) and strontium titanate (SrTiO 3 ). It is evident that the conductivity of both CeO 2 and SrTiO 3 increased with increasing frequency and also obeys Jonscher Equation. In contrast, the conductivity of GO shows frequency independence over the whole frequency window, leading to DC conductivity only. Further, it shows much higher values as compared to CeO 2 and SrTiO 3 . Figure 8c offers the frequency-dependent conductivity of 0.1 wt% CuO-doped CeO 2 compared to those doped with GO (0.15, 0.25, and 0.3 wt%) and SrTiO 3 (0.05 wt%). As evident, the conductivity of GO-doped CeO 2 ceramics is frequency independent up to 10 6 Hz, then significantly increases following the universal power law at higher frequencies. It has been found that the GO-doped CeO 2 ceramics showed higher conductivity values than Cu-doped CeO 2 ceramics. Notably, the highest conductivity (r ac = 2 9 10 -3 ) has been found to composite 2 of Cu:CeO 2 (0.70):GO (0.25):SrTiO 3 (0.05), enabling a novel mechanism for the production of anode materials and a novel fuel cell principle better than reported through literature [53]. The possible underlying mechanism involves the formation of a surface oxygen-deficient layer and core-shell architecture of GO-doped CeO 2 . Also. for these composites, r ac increases with increasing frequency because the excitation of electrons increases with the frequency increase. Further, the observed conductivity decrease occurs at two different rates; it seemed to be nearly perpetual in the low-frequency range, leading to DC conductivity (r dc ), while it considerably increased following the universal power law at higher frequencies (x s ) [54]. This might be due to the hopping of free-charge carriers between different localized states.

Magnetic properties
Undoped CeO 2 and Cu-doped CeO 2 samples' magnetic-field dependency on magnetization (M-H curve) is depicted in Fig. 9a from vibrating sample magnetometer (VSM) measurements at RT. Remarkably, all samples showed very closed M-H curves with coercive fields less than 5 Oe. Also, the average crystallite size obtained from X-ray diffraction analysis (Table 3) is relatively equivalent to the average particle size obtained from TEM analysis (Fig. 2); indicating the formation of single magnetic-domain structures and the presence of superparamagnetic states in our samples. Notably, the undoped CeO 2 nanoparticles exhibited a mixed behavior of weak ferromagnetism at low and diamagnetism at high fields. It also showed a relatively higher M s of 0.003 emu/g at B 5 kOe than reported in the  7.5 9 10 -9 Composite 1 7.5 9 10 -5 Composite 2 2 9 10 -3 Composite 3 5.6 9 10 -4 literature [55,56]. This is a promising result because the bulk CeO 2 is insulating in its origin with Ce 4? in the 4f 0 configuration. Magnetic order in insulating materials originates from owing to the superexchange, and antiferromagnetic ordering exists interaction. However, CeO 2 nanoparticles may show some ferromagnetism because oxygen vacancies can be easily formed during the annealing and crystallization process. Similar outcomes have also been attained in other works [37]. The group showed weak ferromagnetic behaviors, with M S & 0.0019 emu/g at 5 kOe in CeO 2 and some similar oxides, resulting from the superexchange interactions across oxygen vacancies. Regarding Cu-doped CeO 2 , MS increased as Cu content increased, and the most significant MS was noted for x = 0.3, with a value of approximately 0.018 emu/g at 5 KOe. These results confirmed the enhancement of the superexchange interactions of CeO 2 nanoparticles. Based on the electronic configuration of copper 3d 10 4s 1 , we expect the presence of Cu 1? and Cu 2? ions due to the possible formation of 3d 10 and 3d 9 configurations, respectively. Since the d-electrons are paired in the 3d 10 configuration, the Cu 1? ion does not possess a magnetic moment. However, the presence of an unpaired electron in the outer shell of the Cu 2? ion with a 3d 9 configuration contributes to the net magnetization. This strengthens the superparamagnetism in our samples as Cu 2? ion content increases. Figure 9b shows the magnetic-field dependence of M S of the ternary Cu-doped CeO 2 / GO/SrTiO 3 nanocomposites. Results showed a systematic increase in M S as the Cu 2? ion content increased.

Ternary Cu-doped CeO 2 /GO/SrTiO 3 nanocomposites in fuel cell industry
Platinum-based catalysts: Platinum (Pt) is a widely used catalyst material in fuel cells due to its excellent electrocatalytic activity. Compared to Pt-based catalysts, the ternary Cu-doped CeO 2 /GO/SrTiO 3 nanocomposites offer the advantage of lower cost, as Cu is a more economical alternative to platinum. However, Pt-based catalysts still exhibit superior performance in terms of catalytic activity [57]. Nickelbased catalysts: Nickel (Ni) is another commonly used catalyst material in fuel cells. Compared to nickel-based catalysts, the ternary Cu-doped CeO 2 / GO/SrTiO 3 nanocomposites may provide improved stability and durability, as copper oxide (CuO) has been shown to possess enhanced resistance to corrosion and sintering. This could lead to a longer lifespan and improved fuel cell performance [58]. Conductive Supports: GO is often employed as a conductive support material in fuel cell electrode designs due to its high electrical conductivity [59]. The ternary Cu-doped CeO 2 /GO/SrTiO 3 nanocomposites leverage this advantage by incorporating GO. This composite structure facilitates efficient charge transfer and enhances the overall electrical conductivity of the electrode material. CeO 2 : The addition of cerium oxide in the nanocomposites provides various benefits. CeO 2 possesses high oxygen storage capacity and can facilitate oxygen transport within the fuel cell. It also exhibits excellent redox properties, aiding in the oxidation and reduction reactions during fuel cell operation. Incorporating copper into the CeO 2 matrix further enhances its catalytic and electronic properties. Strontium titanate (SrTiO 3 ):SrTiO 3 is a perovskite material known for its high dielectric constant and stability. By incorporating SrTiO 3 into the nanocomposites, the material gains enhanced structural integrity and improved resistance to mechanical stress during fuel cell operation. The presence of SrTiO 3 also contributes to the overall conductivity and stability of the nanocomposites. While the ternary Cu-doped CeO 2 /GO/SrTiO 3 nanocomposites offer advantages such as lower cost, improved stability, and enhanced conductivity compared to certain materials used in fuel cells, they may not match the catalytic activity of platinum-based catalysts. However, the unique combination of copper doping, graphene oxide support, cerium oxide, and strontium titanate in the nanocomposites presents an intriguing avenue for further exploration and optimization in fuel cell applications. It is important to note that these comparisons are general, and further experimental evaluations and performance testing are necessary to provide more precise and quantitative assessments of the ternary Cudoped CeO 2 /GO/SrTiO 3 nanocomposites compared to other materials in the fuel cell industry.

Conclusions
It has been designed to create Ce 1-x Cu x O 2 nanostructures using the sol-gel process. The effect of the Cu ions concentration (0.00 B x C 0.3) on the structure and morphology of the CeO 2 nanocrystals was investigated using TEM, XRD, and optical band gap.
In the crystal structure of cerium oxide, XRD revealed that Cu ions were utterly soluble. Then, a ternary composite of (Cu:CeO 2 ) 0.95-y (GO) y (SrTiO 3 ) 0.05 nanocomposite where (y = 0.15, 0.25, and 0.30) has been carefully built using the grinding technique. AC conductivity, magnetic properties, optical properties, morphological structures, and XRD for graphene oxide, SrTiO 3 , Cu, and/and GO-doped CeO 2 ceramics have indeed been examined concerning frequency and composition. Experimental results showed that the conductivity increases with increasing frequency and obeys the universal power law, i.e., Jonscher Equation. Interestingly, the conductivity of the graphene oxide doped CeO 2 has been dramatically enhanced, which can be helpful in the fuel cell industry. Regarding Cu-doped CeO 2 , MS increased as Cu content increased, and the most significant Ms was noted for x = 0.3, with a value of approximately 0.018 emu/g at 5 KOe. Finally, results showed that the magnetic-field dependence of M S of the ternary Cu-doped CeO 2 /GO/SrTiO 3 nanocomposites increased in M S as the Cu 2? ion content increased.